#------------------------------------------------------------------------------
#$Date: 2019-11-28 18:59:18 +0200 (Thu, 28 Nov 2019) $
#$Revision: 244365 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/23/88/7238805.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7238805
loop_
_publ_author_name
'Wang, XiuLi'
'Xu, Chuang'
'Lin, HongYan'
'Liu, GuoCheng'
'Luan, Jian'
'Chang, ZhiHan'
_publ_section_title
;
 Two novel octamolybdate-based frameworks decorated by flexible
 bis-pyridyl-bis-amide ligands with different spacer lengths
;
_journal_issue                   11
_journal_name_full               'RSC Advances'
_journal_page_first              3592
_journal_paper_doi               10.1039/c2ra22855f
_journal_volume                  3
_journal_year                    2013
_chemical_formula_sum            'C14 H20 Cu Mo4 N4 O18'
_chemical_formula_weight         979.64
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                96.6670(10)
_cell_angle_beta                 94.7390(10)
_cell_angle_gamma                101.7440(10)
_cell_formula_units_Z            2
_cell_length_a                   8.6427(6)
_cell_length_b                   12.3466(9)
_cell_length_c                   12.8266(10)
_cell_measurement_temperature    293(2)
_cell_volume                     1323.02(17)
_computing_structure_refinement  'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0107
_diffrn_reflns_av_sigmaI/netI    0.0199
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            6946
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.70
_exptl_absorpt_coefficient_mu    2.724
_exptl_absorpt_correction_T_max  0.7017
_exptl_absorpt_correction_T_min  0.6399
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    2.459
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             946
_exptl_crystal_size_max          0.18
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.14
_refine_diff_density_max         0.587
_refine_diff_density_min         -0.534
_refine_diff_density_rms         0.083
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.027
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     383
_refine_ls_number_reflns         4642
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.027
_refine_ls_R_factor_all          0.0255
_refine_ls_R_factor_gt           0.0214
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0292P)²+1.3885P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0550
_refine_ls_wR_factor_ref         0.0568
_reflns_number_gt                4154
_reflns_number_total             4642
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2ra22855f.txt
_cod_data_source_block           1
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Triclinic' was changed to
'triclinic' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/RSC/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_database_code               7238805
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu 0.0000 0.5000 -1.0000 0.03629(15) Uani 1 2 d S . .
Cu2 Cu 0.0000 0.0000 -0.5000 0.02805(13) Uani 1 2 d S . .
Mo1 Mo 0.19575(3) -0.02000(2) -1.025322(19) 0.02037(7) Uani 1 1 d . . .
Mo2 Mo -0.06030(3) 0.09884(2) -1.18494(2) 0.02239(8) Uani 1 1 d . . .
Mo3 Mo 0.26004(3) 0.26248(2) -1.05089(2) 0.02801(8) Uani 1 1 d . . .
Mo4 Mo 0.10766(3) 0.17996(2) -0.837260(19) 0.02177(8) Uani 1 1 d . . .
O1 O 0.0292(2) 0.11256(17) -1.00996(15) 0.0218(4) Uani 1 1 d . . .
O2 O 0.0677(2) -0.04917(16) -1.16306(15) 0.0214(4) Uani 1 1 d . . .
O3 O 0.2082(2) 0.02008(17) -0.87310(15) 0.0229(4) Uani 1 1 d . . .
O4 O 0.3294(2) 0.09701(18) -1.05228(17) 0.0281(5) Uani 1 1 d . . .
O5 O 0.1508(3) 0.18412(18) -1.18227(16) 0.0272(5) Uani 1 1 d . . .
O6 O 0.2859(3) 0.25048(18) -0.90269(16) 0.0279(5) Uani 1 1 d . . .
O7 O 0.2927(3) -0.12554(19) -1.03572(18) 0.0318(5) Uani 1 1 d . . .
O8 O -0.1658(3) 0.20021(19) -1.16781(19) 0.0352(5) Uani 1 1 d . . .
O9 O -0.0943(3) 0.04919(19) -1.31638(17) 0.0320(5) Uani 1 1 d . . .
O10 O 0.1559(3) 0.3672(2) -1.04011(19) 0.0445(7) Uani 1 1 d . . .
O11 O 0.4412(3) 0.3247(2) -1.0787(2) 0.0513(7) Uani 1 1 d . . .
O12 O 0.2001(3) 0.19504(19) -0.71270(17) 0.0321(5) Uani 1 1 d . . .
O13 O -0.0058(3) 0.27789(18) -0.83316(18) 0.0323(5) Uani 1 1 d . . .
O14 O 0.5559(4) 0.5486(3) -0.6134(2) 0.0772(11) Uani 1 1 d . . .
O15 O 0.7401(3) 0.2306(2) -0.5246(2) 0.0409(6) Uani 1 1 d . . .
N1 N 0.0999(4) 0.5240(2) -0.8491(2) 0.0387(7) Uani 1 1 d . . .
N2 N 0.5116(4) 0.4077(3) -0.7495(3) 0.0481(8) Uani 1 1 d . . .
H2B H 0.4468 0.3729 -0.8030 0.058 Uiso 1 1 calc R . .
N3 N 0.5339(3) 0.2065(3) -0.6485(2) 0.0421(8) Uani 1 1 d . . .
H3B H 0.4323 0.1872 -0.6632 0.051 Uiso 1 1 calc R . .
N4 N 0.2324(3) 0.0484(2) -0.4454(2) 0.0260(6) Uani 1 1 d . . .
C1 C 0.0180(5) 0.5557(3) -0.7705(3) 0.0465(10) Uani 1 1 d . . .
H1A H -0.0821 0.5699 -0.7869 0.056 Uiso 1 1 calc R . .
C2 C 0.0792(6) 0.5675(4) -0.6660(3) 0.0595(12) Uani 1 1 d . . .
H2A H 0.0204 0.5895 -0.6129 0.071 Uiso 1 1 calc R . .
C3 C 0.2255(6) 0.5471(4) -0.6405(3) 0.0569(12) Uani 1 1 d . . .
H3A H 0.2676 0.5549 -0.5702 0.068 Uiso 1 1 calc R . .
C4 C 0.3101(5) 0.5146(3) -0.7203(3) 0.0447(10) Uani 1 1 d . . .
C5 C 0.2443(5) 0.5057(3) -0.8237(3) 0.0391(9) Uani 1 1 d . . .
H5A H 0.3030 0.4862 -0.8778 0.047 Uiso 1 1 calc R . .
C6 C 0.4714(5) 0.4919(4) -0.6912(3) 0.0509(11) Uani 1 1 d . . .
C7 C 0.6593(5) 0.3714(4) -0.7275(3) 0.0567(12) Uani 1 1 d . . .
H7A H 0.7104 0.4073 -0.6585 0.068 Uiso 1 1 calc R . .
H7B H 0.7304 0.3940 -0.7795 0.068 Uiso 1 1 calc R . .
C8 C 0.6305(5) 0.2464(4) -0.7302(3) 0.0524(11) Uani 1 1 d . . .
H8A H 0.5775 0.2107 -0.7989 0.063 Uiso 1 1 calc R . .
H8B H 0.7320 0.2247 -0.7210 0.063 Uiso 1 1 calc R . .
C9 C 0.5969(4) 0.1992(3) -0.5529(3) 0.0297(7) Uani 1 1 d . . .
C10 C 0.4877(4) 0.1474(3) -0.4785(3) 0.0265(7) Uani 1 1 d . . .
C11 C 0.3298(4) 0.0994(3) -0.5094(2) 0.0261(7) Uani 1 1 d . . .
H11A H 0.2887 0.1026 -0.5780 0.031 Uiso 1 1 calc R . .
C12 C 0.2931(4) 0.0429(3) -0.3471(3) 0.0319(8) Uani 1 1 d . . .
H12A H 0.2272 0.0063 -0.3025 0.038 Uiso 1 1 calc R . .
C13 C 0.4489(4) 0.0892(3) -0.3096(3) 0.0394(9) Uani 1 1 d . . .
H13A H 0.4871 0.0849 -0.2405 0.047 Uiso 1 1 calc R . .
C14 C 0.5479(4) 0.1421(3) -0.3758(3) 0.0358(8) Uani 1 1 d . . .
H14A H 0.6538 0.1739 -0.3520 0.043 Uiso 1 1 calc R . .
O1W O -0.1735(3) 0.3755(2) -0.9700(2) 0.0484(7) Uani 1 1 d . . .
H1WA H -0.1401 0.3270 -0.9378 0.058 Uiso 1 1 d R . .
H1WB H -0.2072 0.3298 -1.0260 0.058 Uiso 1 1 d R . .
O2W O 0.0010(3) 0.15180(19) -0.5226(2) 0.0382(6) Uani 1 1 d . . .
H2WA H -0.0889 0.1696 -0.5209 0.046 Uiso 1 1 d R . .
H2WB H 0.0720 0.2057 -0.4898 0.046 Uiso 1 1 d R . .
O3W O -0.1891(4) 0.7065(3) -0.6300(3) 0.0538(12) Uani 0.768(6) 1 d P A 1
O3W' O -0.2009(12) 0.6599(8) -0.4814(8) 0.038(3) Uani 0.232(6) 1 d P A 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1W Cu1 O1W 180.0 . 2_563
O1W Cu1 N1 88.56(11) . 2_563
O1W Cu1 N1 91.44(11) 2_563 2_563
O1W Cu1 N1 91.44(11) . .
O1W Cu1 N1 88.56(11) 2_563 .
N1 Cu1 N1 180.0 2_563 .
O1W Cu1 O10 91.17(11) . 2_563
O1W Cu1 O10 88.83(11) 2_563 2_563
N1 Cu1 O10 88.85(11) 2_563 2_563
N1 Cu1 O10 91.15(11) . 2_563
O1W Cu1 O10 88.83(11) . .
O1W Cu1 O10 91.17(11) 2_563 .
N1 Cu1 O10 91.15(11) 2_563 .
N1 Cu1 O10 88.85(11) . .
O10 Cu1 O10 179.999(1) 2_563 .
O2W Cu2 O2W 180.0 . 2_554
O2W Cu2 N4 91.22(10) . 2_554
O2W Cu2 N4 88.78(10) 2_554 2_554
O2W Cu2 N4 88.78(10) . .
O2W Cu2 N4 91.22(10) 2_554 .
N4 Cu2 N4 180.0 2_554 .
O7 Mo1 O4 105.82(11) . .
O7 Mo1 O3 102.35(10) . .
O4 Mo1 O3 98.04(9) . .
O7 Mo1 O2 100.76(10) . .
O4 Mo1 O2 96.02(9) . .
O3 Mo1 O2 148.42(8) . .
O7 Mo1 O1 98.28(10) . 2_553
O4 Mo1 O1 155.85(9) . 2_553
O3 Mo1 O1 78.00(8) . 2_553
O2 Mo1 O1 77.64(8) . 2_553
O7 Mo1 O1 172.94(9) . .
O4 Mo1 O1 81.11(9) . .
O3 Mo1 O1 77.63(8) . .
O2 Mo1 O1 76.81(8) . .
O1 Mo1 O1 74.76(8) 2_553 .
O7 Mo1 Mo4 89.49(8) . 2_553
O4 Mo1 Mo4 131.98(7) . 2_553
O3 Mo1 Mo4 123.22(6) . 2_553
O2 Mo1 Mo4 35.98(6) . 2_553
O1 Mo1 Mo4 45.24(5) 2_553 2_553
O1 Mo1 Mo4 84.72(5) . 2_553
O7 Mo1 Mo2 90.25(8) . 2_553
O4 Mo1 Mo2 134.27(7) . 2_553
O3 Mo1 Mo2 36.24(6) . 2_553
O2 Mo1 Mo2 123.17(6) . 2_553
O1 Mo1 Mo2 45.55(5) 2_553 2_553
O1 Mo1 Mo2 85.68(5) . 2_553
Mo4 Mo1 Mo2 89.543(10) 2_553 2_553
O8 Mo2 O9 105.42(12) . .
O8 Mo2 O5 101.94(11) . .
O9 Mo2 O5 98.58(10) . .
O8 Mo2 O3 97.58(10) . 2_553
O9 Mo2 O3 100.50(10) . 2_553
O5 Mo2 O3 147.88(9) . 2_553
O8 Mo2 O1 95.03(10) . .
O9 Mo2 O1 159.40(10) . .
O5 Mo2 O1 79.14(8) . .
O3 Mo2 O1 73.92(8) 2_553 .
O8 Mo2 O2 164.59(9) . .
O9 Mo2 O2 87.52(9) . .
O5 Mo2 O2 83.94(8) . .
O3 Mo2 O2 71.38(8) 2_553 .
O1 Mo2 O2 71.89(7) . .
O8 Mo2 Mo1 85.61(8) . 2_553
O9 Mo2 Mo1 135.65(8) . 2_553
O5 Mo2 Mo1 121.43(6) . 2_553
O3 Mo2 Mo1 35.16(6) 2_553 2_553
O1 Mo2 Mo1 42.29(5) . 2_553
O2 Mo2 Mo1 79.22(5) . 2_553
O11 Mo3 O10 104.84(14) . .
O11 Mo3 O5 105.55(11) . .
O10 Mo3 O5 97.15(11) . .
O11 Mo3 O6 105.15(11) . .
O10 Mo3 O6 96.25(11) . .
O5 Mo3 O6 141.91(9) . .
O11 Mo3 O4 91.96(12) . .
O10 Mo3 O4 163.19(11) . .
O5 Mo3 O4 78.61(9) . .
O6 Mo3 O4 78.35(9) . .
O12 Mo4 O13 104.67(11) . .
O12 Mo4 O6 97.77(10) . .
O13 Mo4 O6 101.82(10) . .
O12 Mo4 O2 101.78(10) . 2_553
O13 Mo4 O2 96.80(10) . 2_553
O6 Mo4 O2 148.54(9) . 2_553
O12 Mo4 O1 160.61(10) . .
O13 Mo4 O1 94.70(9) . .
O6 Mo4 O1 78.75(8) . .
O2 Mo4 O1 74.62(8) 2_553 .
O12 Mo4 O3 87.52(9) . .
O13 Mo4 O3 165.30(9) . .
O6 Mo4 O3 84.30(8) . .
O2 Mo4 O3 72.27(8) 2_553 .
O1 Mo4 O3 73.20(7) . .
O12 Mo4 Mo1 137.36(8) . 2_553
O13 Mo4 Mo1 85.05(8) . 2_553
O6 Mo4 Mo1 121.16(6) . 2_553
O2 Mo4 Mo1 35.60(6) 2_553 2_553
O1 Mo4 Mo1 42.42(5) . 2_553
O3 Mo4 Mo1 80.37(5) . 2_553
Mo1 O1 Mo4 92.34(7) 2_553 .
Mo1 O1 Mo2 92.16(7) 2_553 .
Mo4 O1 Mo2 162.54(10) . .
Mo1 O1 Mo1 105.24(8) 2_553 .
Mo4 O1 Mo1 96.90(7) . .
Mo2 O1 Mo1 98.17(7) . .
Mo1 O2 Mo4 108.42(9) . 2_553
Mo1 O2 Mo2 109.88(9) . .
Mo4 O2 Mo2 104.47(9) 2_553 .
Mo1 O3 Mo2 108.60(10) . 2_553
Mo1 O3 Mo4 109.17(9) . .
Mo2 O3 Mo4 104.73(9) 2_553 .
Mo1 O4 Mo3 120.91(11) . .
Mo2 O5 Mo3 119.06(10) . .
Mo4 O6 Mo3 119.38(11) . .
Mo3 O10 Cu1 170.72(14) . .
C5 N1 C1 118.2(3) . .
C5 N1 Cu1 121.9(2) . .
C1 N1 Cu1 119.8(3) . .
C6 N2 C7 123.5(4) . .
C6 N2 H2B 118.3 . .
C7 N2 H2B 118.3 . .
C9 N3 C8 122.3(3) . .
C9 N3 H3B 118.8 . .
C8 N3 H3B 118.8 . .
C12 N4 C11 118.0(3) . .
C12 N4 Cu2 124.7(2) . .
C11 N4 Cu2 117.0(2) . .
N1 C1 C2 121.5(4) . .
N1 C1 H1A 119.2 . .
C2 C1 H1A 119.2 . .
C3 C2 C1 120.0(4) . .
C3 C2 H2A 120.0 . .
C1 C2 H2A 120.0 . .
C2 C3 C4 118.9(4) . .
C2 C3 H3A 120.6 . .
C4 C3 H3A 120.6 . .
C3 C4 C5 118.7(4) . .
C3 C4 C6 118.4(4) . .
C5 C4 C6 122.8(4) . .
N1 C5 C4 122.6(4) . .
N1 C5 H5A 118.7 . .
C4 C5 H5A 118.7 . .
O14 C6 N2 123.9(4) . .
O14 C6 C4 119.0(4) . .
N2 C6 C4 117.0(3) . .
N2 C7 C8 111.4(3) . .
N2 C7 H7A 109.3 . .
C8 C7 H7A 109.3 . .
N2 C7 H7B 109.3 . .
C8 C7 H7B 109.3 . .
H7A C7 H7B 108.0 . .
N3 C8 C7 112.6(4) . .
N3 C8 H8A 109.1 . .
C7 C8 H8A 109.1 . .
N3 C8 H8B 109.1 . .
C7 C8 H8B 109.1 . .
H8A C8 H8B 107.8 . .
O15 C9 N3 122.5(3) . .
O15 C9 C10 119.8(3) . .
N3 C9 C10 117.6(3) . .
C11 C10 C14 117.9(3) . .
C11 C10 C9 122.5(3) . .
C14 C10 C9 119.6(3) . .
N4 C11 C10 123.3(3) . .
N4 C11 H11A 118.4 . .
C10 C11 H11A 118.4 . .
N4 C12 C13 122.6(3) . .
N4 C12 H12A 118.7 . .
C13 C12 H12A 118.7 . .
C12 C13 C14 119.0(3) . .
C12 C13 H13A 120.5 . .
C14 C13 H13A 120.5 . .
C13 C14 C10 119.3(3) . .
C13 C14 H14A 120.3 . .
C10 C14 H14A 120.3 . .
Cu1 O1W H1WA 114.0 . .
Cu1 O1W H1WB 109.9 . .
H1WA O1W H1WB 93.3 . .
Cu2 O2W H2WA 114.5 . .
Cu2 O2W H2WB 120.9 . .
H2WA O2W H2WB 108.6 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu1 O1W 2.013(3) .
Cu1 O1W 2.013(3) 2_563
Cu1 N1 2.017(3) 2_563
Cu1 N1 2.017(3) .
Cu1 O10 2.364(3) 2_563
Cu1 O10 2.364(3) .
Cu2 O2W 1.928(2) .
Cu2 O2W 1.928(2) 2_554
Cu2 N4 2.016(3) 2_554
Cu2 N4 2.016(3) .
Mo1 O7 1.686(2) .
Mo1 O4 1.745(2) .
Mo1 O3 1.946(2) .
Mo1 O2 1.960(2) .
Mo1 O1 2.157(2) 2_553
Mo1 O1 2.392(2) .
Mo1 Mo4 3.1943(4) 2_553
Mo1 Mo2 3.2030(4) 2_553
Mo2 O8 1.697(2) .
Mo2 O9 1.706(2) .
Mo2 O5 1.907(2) .
Mo2 O3 1.998(2) 2_553
Mo2 O1 2.2882(19) .
Mo2 O2 2.352(2) .
Mo2 Mo1 3.2030(4) 2_553
Mo3 O11 1.684(3) .
Mo3 O10 1.718(3) .
Mo3 O5 1.912(2) .
Mo3 O6 1.922(2) .
Mo3 O4 2.242(2) .
Mo4 O12 1.698(2) .
Mo4 O13 1.704(2) .
Mo4 O6 1.916(2) .
Mo4 O2 1.978(2) 2_553
Mo4 O1 2.2701(19) .
Mo4 O3 2.327(2) .
Mo4 Mo1 3.1943(4) 2_553
O1 Mo1 2.157(2) 2_553
O2 Mo4 1.978(2) 2_553
O3 Mo2 1.998(2) 2_553
O14 C6 1.237(5) .
O15 C9 1.229(4) .
N1 C5 1.333(5) .
N1 C1 1.345(5) .
N2 C6 1.330(6) .
N2 C7 1.454(5) .
N2 H2B 0.8600 .
N3 C9 1.320(4) .
N3 C8 1.461(4) .
N3 H3B 0.8600 .
N4 C12 1.340(4) .
N4 C11 1.341(4) .
C1 C2 1.379(6) .
C1 H1A 0.9300 .
C2 C3 1.361(7) .
C2 H2A 0.9300 .
C3 C4 1.376(6) .
C3 H3A 0.9300 .
C4 C5 1.383(5) .
C4 C6 1.503(6) .
C5 H5A 0.9300 .
C7 C8 1.508(6) .
C7 H7A 0.9700 .
C7 H7B 0.9700 .
C8 H8A 0.9700 .
C8 H8B 0.9700 .
C9 C10 1.502(4) .
C10 C11 1.377(4) .
C10 C14 1.390(5) .
C11 H11A 0.9300 .
C12 C13 1.374(5) .
C12 H12A 0.9300 .
C13 C14 1.379(5) .
C13 H13A 0.9300 .
C14 H14A 0.9300 .
O1W H1WA 0.8500 .
O1W H1WB 0.8501 .
O2W H2WA 0.8501 .
O2W H2WB 0.8500 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O12 Mo4 O1 Mo1 100.1(3) . 2_553
O13 Mo4 O1 Mo1 -77.38(10) . 2_553
O6 Mo4 O1 Mo1 -178.52(9) . 2_553
O2 Mo4 O1 Mo1 18.39(8) 2_553 2_553
O3 Mo4 O1 Mo1 94.10(8) . 2_553
O12 Mo4 O1 Mo2 -155.1(3) . .
O13 Mo4 O1 Mo2 27.4(3) . .
O6 Mo4 O1 Mo2 -73.7(3) . .
O2 Mo4 O1 Mo2 123.2(3) 2_553 .
O3 Mo4 O1 Mo2 -161.1(3) . .
Mo1 Mo4 O1 Mo2 104.8(3) 2_553 .
O12 Mo4 O1 Mo1 -5.6(3) . .
O13 Mo4 O1 Mo1 176.96(9) . .
O6 Mo4 O1 Mo1 75.82(9) . .
O2 Mo4 O1 Mo1 -87.27(8) 2_553 .
O3 Mo4 O1 Mo1 -11.56(6) . .
Mo1 Mo4 O1 Mo1 -105.66(9) 2_553 .
O8 Mo2 O1 Mo1 77.81(10) . 2_553
O9 Mo2 O1 Mo1 -95.5(3) . 2_553
O5 Mo2 O1 Mo1 179.03(9) . 2_553
O3 Mo2 O1 Mo1 -18.64(8) 2_553 2_553
O2 Mo2 O1 Mo1 -93.86(8) . 2_553
O8 Mo2 O1 Mo4 -27.0(3) . .
O9 Mo2 O1 Mo4 159.7(3) . .
O5 Mo2 O1 Mo4 74.2(3) . .
O3 Mo2 O1 Mo4 -123.5(3) 2_553 .
O2 Mo2 O1 Mo4 161.3(3) . .
Mo1 Mo2 O1 Mo4 -104.8(3) 2_553 .
O8 Mo2 O1 Mo1 -176.46(10) . .
O9 Mo2 O1 Mo1 10.3(3) . .
O5 Mo2 O1 Mo1 -75.24(9) . .
O3 Mo2 O1 Mo1 87.09(8) 2_553 .
O2 Mo2 O1 Mo1 11.88(6) . .
Mo1 Mo2 O1 Mo1 105.73(9) 2_553 .
O7 Mo1 O1 Mo1 9.9(8) . 2_553
O4 Mo1 O1 Mo1 178.93(10) . 2_553
O3 Mo1 O1 Mo1 -80.74(9) . 2_553
O2 Mo1 O1 Mo1 80.56(9) . 2_553
O1 Mo1 O1 Mo1 0.0 2_553 2_553
Mo4 Mo1 O1 Mo1 44.95(6) 2_553 2_553
Mo2 Mo1 O1 Mo1 -44.99(6) 2_553 2_553
O7 Mo1 O1 Mo4 104.2(7) . .
O4 Mo1 O1 Mo4 -86.74(9) . .
O3 Mo1 O1 Mo4 13.59(8) . .
O2 Mo1 O1 Mo4 174.89(9) . .
O1 Mo1 O1 Mo4 94.33(9) 2_553 .
Mo4 Mo1 O1 Mo4 139.28(6) 2_553 .
Mo2 Mo1 O1 Mo4 49.34(5) 2_553 .
O7 Mo1 O1 Mo2 -84.6(7) . .
O4 Mo1 O1 Mo2 84.42(9) . .
O3 Mo1 O1 Mo2 -175.25(9) . .
O2 Mo1 O1 Mo2 -13.95(7) . .
O1 Mo1 O1 Mo2 -94.51(9) 2_553 .
Mo4 Mo1 O1 Mo2 -49.56(5) 2_553 .
Mo2 Mo1 O1 Mo2 -139.50(6) 2_553 .
O7 Mo1 O2 Mo4 73.90(12) . 2_553
O4 Mo1 O2 Mo4 -178.70(10) . 2_553
O3 Mo1 O2 Mo4 -62.58(19) . 2_553
O1 Mo1 O2 Mo4 -22.32(9) 2_553 2_553
O1 Mo1 O2 Mo4 -99.32(10) . 2_553
Mo2 Mo1 O2 Mo4 -23.54(12) 2_553 2_553
O7 Mo1 O2 Mo2 -172.49(10) . .
O4 Mo1 O2 Mo2 -65.09(10) . .
O3 Mo1 O2 Mo2 51.02(19) . .
O1 Mo1 O2 Mo2 91.29(9) 2_553 .
O1 Mo1 O2 Mo2 14.29(8) . .
Mo4 Mo1 O2 Mo2 113.61(13) 2_553 .
Mo2 Mo1 O2 Mo2 90.06(8) 2_553 .
O8 Mo2 O2 Mo1 -48.3(4) . .
O9 Mo2 O2 Mo1 164.11(11) . .
O5 Mo2 O2 Mo1 65.20(10) . .
O3 Mo2 O2 Mo1 -93.94(10) 2_553 .
O1 Mo2 O2 Mo1 -15.33(8) . .
Mo1 Mo2 O2 Mo1 -58.43(7) 2_553 .
O8 Mo2 O2 Mo4 67.9(4) . 2_553
O9 Mo2 O2 Mo4 -79.77(10) . 2_553
O5 Mo2 O2 Mo4 -178.67(10) . 2_553
O3 Mo2 O2 Mo4 22.18(8) 2_553 2_553
O1 Mo2 O2 Mo4 100.80(9) . 2_553
Mo1 Mo2 O2 Mo4 57.69(6) 2_553 2_553
O7 Mo1 O3 Mo2 -73.06(12) . 2_553
O4 Mo1 O3 Mo2 178.71(10) . 2_553
O2 Mo1 O3 Mo2 63.11(19) . 2_553
O1 Mo1 O3 Mo2 22.91(9) 2_553 2_553
O1 Mo1 O3 Mo2 99.71(10) . 2_553
Mo4 Mo1 O3 Mo2 24.55(12) 2_553 2_553
O7 Mo1 O3 Mo4 173.30(10) . .
O4 Mo1 O3 Mo4 65.07(11) . .
O2 Mo1 O3 Mo4 -50.53(19) . .
O1 Mo1 O3 Mo4 -90.73(9) 2_553 .
O1 Mo1 O3 Mo4 -13.94(8) . .
Mo4 Mo1 O3 Mo4 -89.09(8) 2_553 .
Mo2 Mo1 O3 Mo4 -113.64(13) 2_553 .
O12 Mo4 O3 Mo1 -163.00(11) . .
O13 Mo4 O3 Mo1 50.6(4) . .
O6 Mo4 O3 Mo1 -64.94(10) . .
O2 Mo4 O3 Mo1 93.80(10) 2_553 .
O1 Mo4 O3 Mo1 15.01(8) . .
Mo1 Mo4 O3 Mo1 58.05(8) 2_553 .
O12 Mo4 O3 Mo2 80.86(10) . 2_553
O13 Mo4 O3 Mo2 -65.6(4) . 2_553
O6 Mo4 O3 Mo2 178.92(10) . 2_553
O2 Mo4 O3 Mo2 -22.35(8) 2_553 2_553
O1 Mo4 O3 Mo2 -101.14(9) . 2_553
Mo1 Mo4 O3 Mo2 -58.10(7) 2_553 2_553
O7 Mo1 O4 Mo3 179.39(11) . .
O3 Mo1 O4 Mo3 -75.26(13) . .
O2 Mo1 O4 Mo3 76.39(12) . .
O1 Mo1 O4 Mo3 3.3(3) 2_553 .
O1 Mo1 O4 Mo3 0.79(11) . .
Mo4 Mo1 O4 Mo3 75.36(14) 2_553 .
Mo2 Mo1 O4 Mo3 -74.20(14) 2_553 .
O11 Mo3 O4 Mo1 178.65(15) . .
O10 Mo3 O4 Mo1 0.9(4) . .
O5 Mo3 O4 Mo1 -75.88(13) . .
O6 Mo3 O4 Mo1 73.58(13) . .
O8 Mo2 O5 Mo3 72.68(14) . .
O9 Mo2 O5 Mo3 -179.45(13) . .
O3 Mo2 O5 Mo3 -53.5(2) 2_553 .
O1 Mo2 O5 Mo3 -20.23(12) . .
O2 Mo2 O5 Mo3 -92.89(12) . .
Mo1 Mo2 O5 Mo3 -19.46(15) 2_553 .
O11 Mo3 O5 Mo2 178.76(14) . .
O10 Mo3 O5 Mo2 -73.62(15) . .
O6 Mo3 O5 Mo2 36.1(2) . .
O4 Mo3 O5 Mo2 89.90(12) . .
O12 Mo4 O6 Mo3 -179.66(13) . .
O13 Mo4 O6 Mo3 -72.83(14) . .
O2 Mo4 O6 Mo3 52.2(2) 2_553 .
O1 Mo4 O6 Mo3 19.68(12) . .
O3 Mo4 O6 Mo3 93.64(12) . .
Mo1 Mo4 O6 Mo3 18.52(15) 2_553 .
O11 Mo3 O6 Mo4 -178.34(14) . .
O10 Mo3 O6 Mo4 74.41(15) . .
O5 Mo3 O6 Mo4 -35.6(2) . .
O4 Mo3 O6 Mo4 -89.47(13) . .
O11 Mo3 O10 Cu1 -133.2(10) . .
O5 Mo3 O10 Cu1 118.5(10) . .
O6 Mo3 O10 Cu1 -25.7(10) . .
O4 Mo3 O10 Cu1 44.4(12) . .
O1W Cu1 O10 Mo3 -45.9(10) . .
O1W Cu1 O10 Mo3 134.1(10) 2_563 .
N1 Cu1 O10 Mo3 -134.5(10) 2_563 .
N1 Cu1 O10 Mo3 45.5(10) . .
O10 Cu1 O10 Mo3 -113(17) 2_563 .
O1W Cu1 N1 C5 115.3(3) . .
O1W Cu1 N1 C5 -64.7(3) 2_563 .
N1 Cu1 N1 C5 87(7) 2_563 .
O10 Cu1 N1 C5 -153.5(3) 2_563 .
O10 Cu1 N1 C5 26.5(3) . .
O1W Cu1 N1 C1 -62.3(3) . .
O1W Cu1 N1 C1 117.7(3) 2_563 .
N1 Cu1 N1 C1 -90(7) 2_563 .
O10 Cu1 N1 C1 28.9(3) 2_563 .
O10 Cu1 N1 C1 -151.1(3) . .
O2W Cu2 N4 C12 117.6(3) . .
O2W Cu2 N4 C12 -62.4(3) 2_554 .
N4 Cu2 N4 C12 -19(2) 2_554 .
O2W Cu2 N4 C11 -55.7(2) . .
O2W Cu2 N4 C11 124.3(2) 2_554 .
N4 Cu2 N4 C11 167(2) 2_554 .
C5 N1 C1 C2 -1.0(5) . .
Cu1 N1 C1 C2 176.7(3) . .
N1 C1 C2 C3 0.0(6) . .
C1 C2 C3 C4 0.0(7) . .
C2 C3 C4 C5 1.0(6) . .
C2 C3 C4 C6 -179.8(4) . .
C1 N1 C5 C4 2.1(5) . .
Cu1 N1 C5 C4 -175.6(2) . .
C3 C4 C5 N1 -2.1(5) . .
C6 C4 C5 N1 178.7(3) . .
C7 N2 C6 O14 0.9(6) . .
C7 N2 C6 C4 -176.3(3) . .
C3 C4 C6 O14 -34.7(5) . .
C5 C4 C6 O14 144.4(4) . .
C3 C4 C6 N2 142.7(4) . .
C5 C4 C6 N2 -38.2(5) . .
C6 N2 C7 C8 132.0(4) . .
C9 N3 C8 C7 -88.7(5) . .
N2 C7 C8 N3 -63.4(4) . .
C8 N3 C9 O15 3.8(6) . .
C8 N3 C9 C10 -174.6(3) . .
O15 C9 C10 C11 -172.6(3) . .
N3 C9 C10 C11 5.8(5) . .
O15 C9 C10 C14 4.2(5) . .
N3 C9 C10 C14 -177.4(3) . .
C12 N4 C11 C10 -0.9(5) . .
Cu2 N4 C11 C10 172.9(2) . .
C14 C10 C11 N4 0.1(5) . .
C9 C10 C11 N4 176.9(3) . .
C11 N4 C12 C13 1.3(5) . .
Cu2 N4 C12 C13 -171.9(3) . .
N4 C12 C13 C14 -0.9(6) . .
C12 C13 C14 C10 0.1(5) . .
C11 C10 C14 C13 0.4(5) . .
C9 C10 C14 C13 -176.5(3) . .
